Experimental Study on Mechanical Properties of Interface between Basalt Fiber-Reinforced Polymer/Glass Fiber-Reinforced Polymer Composite Cement Plate and Concrete

The bonding behaviors of the plate-concrete interface of a composite structure consisting of a concrete block in the middle and two cement plates at both sides play a key role in its overall mechanical performance. In this paper, the authors conduct 3 groups of push-out shear tests on a total of 39 composite samples to assess the bonding performance. The inﬂuence of the FRP cement plates, the concrete strength, and the ribs installed in the cement plate on the interfacial shear strength, the relative bond-slip, strain, and the failure modes of the composite samples is recorded and analyzed. The results show that (1) the shear strength and bond-slip performance of the interface are largely improved if the GFRP/BRRP cement plates are used; (2) shear strength of the interface increases with the concrete strength, while the deformation behaviors show no signiﬁcant improvement; (3) an inclusion of the ribs to the interface enhances the shear strength and shear stiﬀness but decreases the maximum relative slip at failure; (4) most of the samples present the shear failures along the interface; however, the bending shear failure prior to the interface shear failure is also observed on the concrete block for low concrete strength samples and the samples with ribs; and (5) regression method is used to develop a constitutive model of the stress-slip at the interface to describe the relationship between the shear strength with the cement plates, the concrete strength, and ribs.


Introduction and Background
e fiber-reinforced polymer (FRP) material has become one of the most popular construction materials and has been widely used in civil engineering in recent years [1,2]. As compared to traditional materials, the FRP material has higher strength, lighter weight, easier construction procedures, and more reliable performance. Of the FRP materials, the glass fiber-reinforced polymer (GFRP) and the basalt fiber-reinforced polymer (BFRP) are two of the most commonly used fiber materials. e lightweight GFRP has a long service life, good corrosion resistance, and many other advantages. e electric-insulating BFRP also shows good resistance to corrosion as well as to high temperature [3,4]. Both the two types of new FRP materials have become the most important materials in structure strengthening engineering [5,6]. is paper has utilized the BFRP/GFRP materials for the construction of a composite structure. e composite structure consists of a concrete block in the middle and two FRP reinforced cement plates at both sides (see Figure 1). e cement plate is reinforced with the fiber mesh and can be used as a permanent mold/plate. e concrete is poured between the two permanent plates during construction; thus, a composite structure is easily created. As compared to the traditional cement plates, the permanent composite plate offers advantages in terms of the overall costs, the construction period, and materials saving including steel, wood, and bamboo. It also saves demolding operations and transportation cost. As a composite structure, both the middle concrete and the reinforced composite cement plates at two sides can sustain loads, and therefore, the overall mechanical performance is improved. However, the bonding performance between the reinforced permanent plates and concrete becomes the major concern for this composite structure.
From the field application of the composite structures, it is observed that the early separation of the FRP reinforced cement plates from the concrete block greatly impairs the load-bearing capacity of the composite structure. erefore, extensive studies have been made to investigate the bonding behaviors of the concrete-plate interface. Ma et al. performed the simple shear tests to study the bonding properties of a concrete beam reinforced by CFRP sheets under the cyclic loading condition [7]. ey found that the length and thickness of the CFRP sheets and the concrete grade have a major impact on the bonding between the CFRP sheets and the concrete and that a larger loading rate reduces the fatigue endurance of the interface. Chen et al. reinforced the manually precracked single trabeculae by attaching FRP sheets on its sides and tested the bonding performance [8].
e influence of dimensions of the FRP sheets and the applied loading conditions were included in their work. Nanni et al. studied the interfacial bonding performance of the interface between FRP reinforced laminated plates and the middle concrete and found that the stiffness of the laminated plate significantly impacts the failure load of the interface [9]. Nakaba et al. proposed a constitutive model to describe the relationship between the local bond stress and the slip at the interface between the FRP reinforced laminated plate and the concrete based on a number of double shear tests [10]. Li et al. performed the simple shear tests on the concrete samples with embedded CFRP sheets [11]. e length of the embedding CRFP sheets was found to have a great influence on the bonding behaviors.
Other researchers improved the bonding performance of the composite structures by material modification and the connection modes at the interface. Gravina et al. investigated the bonding behavior between the FRP laminated sheets preimpregnated with resin [12]. e resin was also used for concrete modification and the thickness of the bonding interface was included in their experiment to study the adhesive performance of the composite structure. e material modification can improve the bonding force. Zhou et al. improved the bonding properties of the composite structure by increasing the mechanical fastening pressures between the FRPconcrete interfaces [13]. Chen et al. designed a horizontal slot at the interface to improve the bonding and deformation capacity of the composite structure [14]. Studies on the endurance of the interface were also documented in previous works. Wang et al. concluded that the bonding force between the FRP plates and the concrete was reduced when subjected to water, seawater, high temperature, the cyclic damp heat condition, and the corrosion under acid and alkali conditions [15]. ey found from their tests that the high temperature presented worse deterioration to the interface properties than the low temperature and the presence of mortar joint in the composite structure further reduced the bonding capacity of the interface. e endurance of the composite structure interface under the extreme weather and loading conditions was included in Wang et al. [16]. e bonding between the FRP cement plates and the concrete is the key factor largely determining the overall performance of the composite structures. A number of researchers have developed the constitutive models to describe the bonding stress and slip deformation at the interface. Lin and Cao investigated the bonding performance at the pure bending section of the CFRP concrete structure and developed an analytical model to describe the bond and slip behaviors at the interface [17]. Woo [23]. e model was used to predict the separation of the interface. Ko et al. conducted the double shear tests on 18 composite samples to investigate the bonding between the GFRP sheets and the concrete, based on which a bilinear stress-slip model was proposed [24]. Hao et al. performed the pull-out tests to study the bonding between the steel strand and the concrete on 180 samples, with a consideration of the placement of the strand and the dimensions of the concrete [25]. ey improved their bondingslip constitutive model based on the experimental results. e previous studies have improved our understandings of the bonding performance of the composite structures between the FRP materials and the concrete. However, the CFRP and GFRP sheets rather than the FRP cement plates were used for most of the composite structures in previous works.
is paper attempts to evaluate the bonding performance between the BFRP/GFRP reinforced cement plates and the concrete block with a consideration of the types of the fiber mesh, the concrete grade, and the inclusion of steel ribs in the cement plates. ree sets of experiments were designed and were used to conduct the push-out tests in the present work. e first set compares the bonding performance of the composite structures with three different cement plates, that is, the regular cement plates for the GS samples, the BFRP reinforced plates for the GB samples, and the GFRP reinforced plates for the DG samples. e second set consists of different composite structures made of the C15, C30, and C50 concrete. e third set includes the composite samples with and without ribs to investigate the influence of the mechanical interaction at the interface. e failure characteristics of the composite samples and the relation between the shearing capacity and the slip deformation at the interface were recorded. e shearing strength as a function of the slip deformation was obtained using the regression approach. e results from this paper may provide a reference for improving the bonding performance and promoting the industrial applications of the composite structures.

Sample Preparation.
In this research, the push-out shear test is performed to study the influence of the fiber-reinforced cement plate, concrete strength, and ribs in the plate on the bonding performance of the plate-concrete interface. Figure 1 gives a front view of the composite structure. e cement plate at both ends is 20 mm thick, 150 mm high, and 150 mm long, and the middle concrete body is 110 mm thick, 120 mm high, and 150 mm long. erefore, the overall dimension of the composite specimen prepared in this study is 150 × 150 × 150 mm. Efforts were made during the sample construction to make sure that all specimens have the same size. e concrete is poured 30 mm above the bottom; thus, the push-out shearing test can be performed. e cement plate is constructed using cement, fly ash, expanded perlite, sand, water reducing agent, and coupling agent with a proportion of 1 : 0.25 : 0.015 : 0.15 : 0.007 : 0.015 by weight. During construction, the GFRP plate uses low alkalinity cement while the BFRP plate uses the Portland cement [26]. Fiber meshes are placed on both side surfaces of the plate. e fiber meshes used in the GFRP and BFRP plates have the same density (160 g/m 2 ). e construction of the BFRP and GFRP composite samples includes three procedures: (1) preparation of the experimental mold and cement slabs; (2) concrete pouring between the composite cement plates; and (3) sample curing at room temperature for 28 days. For ease of demolding, the inner surface of the mold was cleaned and coated with lubricating oil before pouring. Two pieces of cement plates are placed at both sides of the mold, and a 30 mm thick foam block is placed at the bottom between the two plates for reserving space for the later push-out test. e foam is tightly pressed on cement plates to prevent slurry leakage. e concrete is poured at a designed strength (i.e., C15, C30, and C50 in this study) for comparing the concrete strength influence on the bonding behaviors of the plate-concrete interface. After demolding, the composite samples are cured for a period of 28 days at room temperature.

Loading Condition and Data Measuring System.
e push-out shearing test is performed on a compression testing machine. Figure 2 plots the loading condition of the composite sample. e composite sample is placed between the upper and lower bearing plates. A steel plate slightly less than 110 mm wide is put between the upper bearing plate and the sample for performing the push-out shearing test. e test is ceased when the sample is damaged. e bonding performance of the plate-concrete interface (including the shear strength and relative bond-slip) is the major concern of this study. e layout of the measuring points is also shown in Figure 1. A total of 3 displacement measuring points can be found on the left and right sides of the two plates and on the front surface of the concrete body, respectively. e relative slip of the plate-concrete interface can therefore be obtained. e strain data of the interface, however, were measured by 2 strain gauges placed at the plate-concrete boundaries. e testing machine (type SANS) is used to load, the sensor (type CFBLY) is used to record the load data, and the data acquisition system (type BETC) is used to collect data. e shear stress, relative movement, and strain data of the interface are recorded during the test. e failure characteristics and development of fractures on the sample are also observed by a camera.

Effect of Fiber Mesh Type on Interface Bonding
Performance. As mentioned above, the inclusion of fiber mesh in the cement plate and its type should influence the bonding performance of the plate-concrete interface. erefore, the first group of tests compares the influence of three kinds of cement plates, that is, the plain Portland  cement plate without fiber reinforcement (GS); BFRP reinforced ordinary Portland composite cement plate (GB), and GFRP reinforced low alkalinity composite cement plate (DG). All the three sets of composite specimens utilize C30 for the middle concrete during the sample preparation. In each set, 3 samples are prepared. erefore, the total number of samples in this group is 9. e samples are assigned with different numbers for better analysis. Sample GS C30-1, for instance, represents the first sample with the GS cement plates on both sides and C30 middle concrete. Figure 3 shows the failure characteristics of the samples after the shear test. It is found that all 3 GS samples present brittle failure (see Figure 3 e shearing test reveals that the fiber-reinforced composite sample fails along the plate-concrete interface prior to the cement plate, indicating that the overall loadbearing capacity of the cement plate is largely improved by the fiber materials. e bonding performance of the interface is also enhanced for the fiber-reinforced samples as compared to the nonfiber samples and the interfacial shear strength of the fiber-reinforced sample is even higher than that of C30 concrete itself. Table 3 compares the shear strength of the plate-concrete interface for the composite samples with different fiber-reinforced cement plates. e shear strength of the nonfiber composite sample (GS samples) is noticeably lower than the fiber-reinforced samples. e mean value of the shear strength for the GS samples is 0.64 MPa, which is only 63.63% and 55.77% of the GB (1.00 MPa) and DG (1.14 MPa) composite samples, respectively. Hence, the fiber mesh significantly improves the shear strength of the plate-concrete interface. It is also noted that DG composite samples with GFRP cement plates have a slightly larger shearing performance than the GB samples with BFRP plates. Table 4 lists the maximum relative slip of the plate-concrete interface with different fiber meshes. e average displacement values of the GS, GB, and DG composite samples are 0.27, 0.54, and 0.45 mm, respectively. erefore, the composite samples with fiber-reinforced plates allow a larger relative displacement on the plate-concrete interface compared to the composite samples with nonfiber plates. Figure 4 plots the relationship of the shearing stress over the relative displacement. It shows that the shearing stresses of the GB and DG composite samples increase at a large and similar rate. e fast growth of shearing stresses ends when the relative displacement is about 0.14 mm. e stresses then reach a plateau and only increase slightly over a large displacement; that is, the interface of the fiber-reinforced samples shows plastic deformation characteristics. e slope of the curve for the GS sample, however, is much lower. erefore, the fiber-reinforced cement plate also improves the deformation performance of the interface. Table 5 summarizes the maximum and mean strain values of the interface for the 3 sets of samples. It shows that the mean strain value of GS C30 samples is only 10.6% of GB C30 and 18% of DG C30 samples. e mean maximum strain of GB C30 samples is 1.7 times that of DG C30 specimen. e shearing stress-strain curve is given in Figure 5. An approximately linear relationship is observed between the stress and strain for all the three sets of samples. It can also be found from the curves that the GB and DG samples show some plastic behaviors at the later stage, which corresponds to the stress-displacement curves.

Effect of Concrete Strength on Interface Bonding
Performance.
e bonding performance of the plate-concrete interface is also influenced by the concrete strength.
e composite samples in this group use C15, C30, and C50 for middle concrete, respectively. e cement plates at both sides are BFRP reinforced ordinary Portland composite cement plate (GB) and GFRP reinforced low alkalinity composite cement plate (DG). erefore, this group of experiments prepares 6 sets of tests with 18 samples in total. Each sample is assigned a unique number. For instance, the composite structure with BFRP cement plates and C15 concrete has 3 samples, that is, GB C15-1, GB C15-2, and GB C15-3. Figure 6 gives the fracture development and failure characteristics of the samples after the test. Note that the GB C30 and DG C30 samples have   Figure 3. us, Figure 6 only shows the results of the C15 and C30 samples. It is observed that most of the GB samples see shear failure along the interface, except the GB C30-1 and GB C50-3 with failures also observed on the concrete body. GB C30-1 finds failure on both the cement plate and the middle concrete rather than fails in shear along the interface (Figure 3(b)). e GB C50-3 sample, however, finds tensile damage on top of the sample beside the shear failure along the interface (Figure 6(b)).

Failure Modes of Specimens.
By comparison, the DG samples show different failure modes. Samples DG C15-1 and C15-3 find tensile failure in the middle concrete due to bending (see Figure 6(c)). e fracture initiates from the bottom of the concrete and extends upwards. Sample DG C15-2, however, sees the common shear failure along the plate-concrete interface; that is, the middle concrete separates from the cement plate when the limit relative displacement is reached. Likewise, all the DG C30 and C50 samples fail in shear along the concrete-plate interface (see Figures 3(c) and 6(d)). e DG C50-3 sample shows a slightly different failure mode, although with the fracture first developing along the interface and then extending to the concrete before cutting through the entire sample.

Advances in Materials Science and Engineering
From the above analysis, we learn that most of the failure occurs in shear along the interface. However, it is also interesting to note that bending shear failure in concrete is observed for Samples DG C15-1 and C15-3, and compression shear failure on both cement plate and concrete is found in Sample GB C30-1. In other words, failure in the concrete or cement plate may occur prior to the interfacial shear failure, indicating that the shear strength of the interface may be larger than the cement plate and the concrete body, especially when the concrete strength is low (say, the C15 samples).

Relative Bond-Slip of the Interface.
e maximum relative bond-slip along the concrete-plate interface is provided in Table 7. It is noticed that the relative displacement of the interface shows no significant difference.
is differs from the positive relationship between the shear strength and the concrete strength.  Figure 7 plots the shearing stress-relative displacement curves for composite samples with different cement plates and concretes. e deformation behavior along the interface shows different characteristics for samples with different concrete strength, although the maximum relative displacements are generally the same. It shows that the shearing stress for C30 and C50 samples increases rapidly at the early stage of loading, which means the samples pick up the shear load quickly but at a small displacement. After the relative displacement reaches about 0.14 mm, the C30 and C50 samples reach a plateau and show clear plastic deformation behavior, with a large amount of displacement but a small increase in shearing stress. By comparison, the C15 sample shows an approximately linear relationship between the shearing stress and the displacement. It is also observed from the slope of the curves that the overall shearing stiffness of the composite samples is increased with the increase of concrete strength. Table 8 gives the maximum and mean values of the interface strain. Figure 8 shows the shearing stress-strain curves. It is observed that the interfacial shearing stiffness and deformation performance for both GB and DG samples are increased with enhanced concrete strength. In particular, the C50 samples show obvious plastic displacement behavior at the late stage of loading. e maximum strain, however, does not show a specific relationship with relation to the concrete strength. is is consistent with the results of the interface slip test, which shows that the interface deformation properties can also be reflected by measuring the interfacial strain.

Effect of Rib on Interface Bonding
Performance. e addition of ribs in the cement plate and its layout are also influential to the bonding performance of the plate-concrete interface.
e authors have designed cement plates with horizontal (HL) and vertical (ZL) ribs, which are compared to the nonrib samples (WL). e rib is 10 mm in width and 5 mm in height. A total of 2 ribs are symmetrically placed in the cement plate with a spacing of 100 mm. During construction, the BFRP (GB) and GFRP (DG) materials are used for cement plates and C30 for concrete. e sample ID is assigned to each sample. Sample GB HL-1 represents the first sample with BFRP cement plate and HL rib. Figure 9 plots the failure characteristics of the samples after the test. All the 3 GB HL samples see shear failure near the plate-concrete interface in both the cement plate and the concrete (Figure 9(a)). is differs from the smooth shear failure of the interface and complete separation of the plate and concrete for the WL samples. e GB ZL samples also see shear failure along the plate-concrete interface (Figure 9(b)). However, fractures extend towards the middle concrete and damage is found in the concrete at top of the sample, especially for the GB ZL-3 sample.

Failure Modes of Specimens.
Shear failure along the interface is observed for Samples DG HL-1 and DG HL-2 (Figure 9(c)). e middle concrete for Sample DG HL-1 also sees shear failure near the failure interface side at the top. DG HL-3, however, fails in bending shear in the concrete. e bending shear crack initiates from the bottom and extends upward to the top surface, but the interfaces on both sides still remain intact. Similar to the GB ZL samples, the DG ZL samples find shear failure along the interface and splitting failure on the concrete at the top.      Advances in Materials Science and Engineering Sample DG ZL-3, however, shows an inclined compression shear failure mode with a 45°fracture (in relation to the interface) developing upward obliquely from the bottom edge (Figure 9(d)). Table 9 summarizes the maximum shear load of the interface and the shear strength at failure. It is obvious that the samples with ribs in the plate present much larger shear strength than the nonrib ones. e shear strength values for the rib samples almost double those for the nonrib. is is because the presence of ribs in the cement plate not only increases the bonding area but also improves the load transmission between the cement plate and the concrete. e ribs provide extra mechanical interaction at the interface rather than the pure friction for WL samples. erefore, the ribbed samples are more reliable.

Shear Strength of the Interface.
It is also noted that the samples with HL ribs have better interface bonding performance compared to the samples with ZL ribs. e HL ribs play a more important part than the ZL ribs in improving the mechanical interaction at the interface.

Relative Bond-Slip of the Interface.
e maximum relative bond-slip of the interface is listed in Table 10 and the curve of the interfacial shear stress-relative displacement is shown in Figure 10. It can be seen that, due to the mechanical interlocking between the rib and the concrete, not only is the interfacial shear bearing capacity of the composite samples increased, but also the interfacial shear stiffness of the composite samples is greatly increased, the HL rib samples present the largest shearing stiffness. e maximum interface slip of the samples after being ribbed is significantly reduced. e sample with HL ribs has the lowest relative displacement, followed by the ZL rib sample and the WL sample. It is also observed that no plastic deformation behavior is found for the rib samples. Table 11 gives the maximum strain of the interface at failure. e WL samples have the highest strain values, while the ribbed samples show significant lower strain. e stressstrain curves are plotted in Figure 11. e HL rib sample has the largest shear modulus and the ZL rib sample is the second, while the WL sample has the lowest shear modulus. e ribs at the interface increase the mechanical friction of the sample but allow less relative movement, which is consistent with the previous results of interfacial bond-slip tests.

Regression Expression for the Shear Strength of the
Interface. e influence of the cement plate, concrete strength, and rib on the bonding performance of the interface has been studied using the push-out shear test in this paper. e regression analysis is then utilized to establish a mathematical relation between the shear strength and the 3 influencing factors, which is given in equation (1): where τ u is the shear strength of the plate-concrete interface in MPa; α is a dimensionless factor representing the influence of the fiber mesh type (α �1 for the nonfiber cement plate, α � 1.793 for the GFRP cement plate, and α � 1.572 for the BFRP cement plate); c is also dimensionless expressing the influence of rib in the cement plate (c �1 for WL sample, c � 2.244 for the sample with HL rib, and c � 1.977 for the ZL rib); f cuk is the standard cube compressive strength of the concrete. e shear strength of the plate-concrete interface is computed using equation (1).

A Constitutive Model for the Shear Strength-Relative Slip of the Interface
According to the test results, all the samples show a linear relationship between the shear strength and the relative slip at the early loading stage. After reaching the maximum, the shear strength plateaus over a long relative displacement, but only for the samples with fiber-reinforced nonrib cement plates. However, for the nonfiber, nonrib samples, or the ribbed samples with no fiber-reinforced cement plates, the stress-slip curve only has the rising linear stage, and there is no obvious plastic deformation stage. ese samples fail after the peak shear strength is reached and no plastic behavior is observed. Figure 12 is used to express the relationship of the shearing stress and relative slip, where τ is the shearing stress in MPa and S is the value of the relative slip in mm. e shear stress of the interface increases linearly with the relative displace before it reaches the characteristic value of the relative displacement, S 0 . e shear stress then maximizes at τ u over the displacement range of S 0 <S < S u . e curve is divided into elastic (OA) and plastic (AB) sections according to the load-deformation characteristics. Note that only the linear growth Section OA is used for expressing the stressdisplacement relationship for the nonfiber and ribbed  samples.
e load-deformation behavior of the samples using fiber-reinforced cement plates includes both sections.

Elastic Behavior of the Sample (Section OA).
e experimental data are used to obtain the mathematical relationship between the shearing stress and relative slip using the regression method. Equation (2) gives the expression for the linear growth of stress over displacement in Section OA.
where τ is the shear stress of the plate-concrete interface; β is the dimensionless factor concerning the influence of fiber mesh on the stress-slip relationship (β �1 for the nonfiber cement plate, β � 2.633 for the GFRP cement plate, and   Figure 12: Constitutive model for the shearing stress-relative slip of the interface. β � 2.619 for the BFRP cement plate); η is a dimensionless parameter explaining the influence of rib in the cement plate (η �1 for WL sample, η � 1.735 for the sample with HL rib, and η � 1.304 for the ZL rib); f cuk is the standard cube compressive strength of the concrete; S is the relative slip of the plate-concrete interface (0 <S < S 0 ).

Plastic Behavior of the Sample (Section AB).
In the following section of the curve, the shear stress of the interface maximizes at τ u while the relative slip continues to increase. Equation (3) shows the relationship of shear stress over the relative slip.
where τ u is the shear strength of the interface. e shear strength can be obtained using equation (1).

Characteristic
Value of the Relative Slip. S 0 is the characteristic value of relative slip referring to the amount of relative displacement when the shear stress reaches its peak value. Combining equations (1) and (2) yields the expression for S 0 : In Figure 12, S u represents the maximum relative displacement when the samples fail completely. Note that, for the samples without plastic behavior, S u � S 0 and is normally less than 0.3 mm. For samples with plastic behavior, however, the relative slip characteristic values fall in the range of 0.45-0.55 mm.
It should be noted that the maximum concrete strength in this study uses the C50. Hence, the obtained equations above only apply for C50 concrete or less, and further research needs to be done for concrete strength grade higher than C50.

Summaries and Conclusions
is paper has analyzed the bonding performance of the plate-concrete interface by performing push-out shear test in the laboratory. A total of 3 groups of experiments have been conducted to assess the influence of the fiber mesh type, the concrete strength, and the inclusion of ribs in the cement plate. e failure characteristics of the sample, shear strength of the interface, and the relationship of load-deformation have been discussed for different samples. e regression method is adopted to compute the shear strength and the stress-displacement slip of the interface using the experimental data. e results provide guidance for improving the bonding performance of the interface. Important findings of this paper are listed as follows: (1) Instead of brittle failure, the composite sample with fiber-reinforced cement plate shows plastic behavior following the elastic stage. e deformation performance of the interface is therefore improved by using the fiber-reinforced cement plate. ese fiber-reinforced cement plates increase not only the buckling strength but also the shear stress of the plate-concrete interface.
ere is no appreciable difference between the GFRP and BFRP composite samples, although the GFRP samples have slightly larger shear strength, while the BFRP samples show slightly better deformation performance.
(2) e shear strength of the plate-concrete interface is improved when using higher strength of concrete. However, the maximum relative slip at failure is not increased with the increase of concrete strength.
Composite samples with larger concrete strength (say C50) show good shear stiffness and plastic behavior following the elastic stage. (3) e shear strength and shear stiffness of the interface are largely improved by setting ribs in the cement plate. However, the maximum relative slip of the interface is decreased for the rib samples. e layout of the rib is also influential to the interface bonding performance. e HL rib has larger shear strength and stiffness but lower maximum displacement. (4) Good consistency is found between the stress-strain and stress-slip relationship of the interface. erefore, the deformation characteristics of the interface can also be represented by measuring the strain data. (5) e regression analysis gives the mathematical expression for the shear strength and the constitutive relationship of the stress-slip of the interface. e approximate elastic-perfectly plastic behavior is found for the samples using fiber-reinforced cement plates, while only linearly elastic behavior is observed for both nonfiber and rib samples.

Abbreviations
Sp1, Sp2, and Sp3: Specimens 1, 2, and 3 τ: Shear stress of the plate-concrete interface τ u : Shear strength of the plate-concrete interface S: Relative bond-slip of the plate-concrete interface S 0 : Characteristic value of relative bond-slip when the shear stress reaches maximum S u : Maximum relative bond-slip when the samples fail completely f tk : Standard cube compressive strength of the concrete α: A dimensionless factor representing the influence of fiber mesh type on shear strength c: A dimensionless factor expressing the influence of rib on shear strength β: A dimensionless factor concerning the influence of fiber mesh on stress-slip relationship η: A dimensionless factor concerning the influence of rib on stress-slip relationship.

Data Availability
e data used to support the findings of this study are included within the article.

Conflicts of Interest
e authors declare no conflicts of interest.